Coble creep

Coble creep
‎A diagram showing how atoms and vacancies move through a grain as the mechanism of Coble creep

Coble creep, a form of diffusion creep, is a mechanism for deformation of crystalline solids. Coble creep occurs through the diffusion of atoms in a material along the grain boundaries, which produces a net flow of material and a sliding of the grain boundaries.

Coble creep is named after Robert L. Coble, who first reported his theory of how materials creep over time in 1962 in the Journal of Applied Physics[1].

The strain rate in a material experiencing Coble creep is given by:

$\frac{d\epsilon}{dt}= \frac{\sigma}{d^3} D_{gb} e^{-Q_{Coble}/RT}$

where

• σ is the applied stress
• d is the average grain boundary diameter
• Dgb is the diffusion coefficient in the grain boundary
• QCoble is the activation energy for Coble creep
• R is the molar gas constant
• T is the temperature in kelvins

Note that in Coble creep, the strain rate $\frac{d\epsilon}{dt}$ is proportional to the applied stress σ; the same relationship is found for Nabarro-Herring creep. However, the two mechanisms differ in their relationship between the strain rate and grain size d. In Coble creep, the strain rate is proportional to d − 3, whereas the strain rate in Nabarro-Herring creep is proportional to d − 2. Researchers commonly use these relationships to determine which mechanism is dominant in a material; by varying the grain size and measuring how the strain rate is affected, they can determine the value of n in $\frac{d\epsilon}{dt}~\alpha ~d^n$ and conclude whether Coble or Nabarro-Herring creep is dominant[1].

References

(1) Meyers and Chawla (1999): "Mechanical Behavior of Materials," 555-557.

Wikimedia Foundation. 2010.

Look at other dictionaries:

• Creep (deformation) — For other uses, see Creep (disambiguation). v · d · e Materials failure modes Buckling …   Wikipedia

• Diffusion creep — refers to the deformation of crystalline solids by the diffusion of vacancies through their crystal lattice.[1] Diffusion creep results in plastic deformation rather than brittle failure of the material. Diffusion creep is more sensitive to… …   Wikipedia

• Deformation mechanism — In structural geology, metallurgy and materials science, deformation mechanisms refer to the various mechanisms at the grain scale that are responsible for accommodating large plastic strains in rocks, metals and other materials. Contents 1… …   Wikipedia

• Grain growth — refers to the increase in size of grains (crystallites) in a material at high temperature. This occurs when recovery and recrystallisation are complete and further reduction in the internal energy can only be achieved by reducing the total area… …   Wikipedia

• Kornwachstum — tritt in polykristallinen Festkörpern auf. Bei genügend hohen Temperaturen und sobald Kristallerholung und Rekristallisation vollständig stattgefunden haben, kann eine weitere Absenkung der inneren Energie nur noch über eine Verkleinerung der… …   Deutsch Wikipedia

• Pantomime — For other uses, see Pantomime (disambiguation). The Christmas Pantomime colour lithograph bookcover, 1890, showing the harlequinade characters Pantomime (informally, panto) not to be confused with a mime artist, a theatrical performer of mime is… …   Wikipedia

• Opposition to the War in Afghanistan (2001–present) — Foreign troops forcibly breaking into an Afghan home to conduct a house search, with a woman and child in the background. Opposition to the decade long Afghanistan war stems from numerous factors these include the view that the U.S. invasion of… …   Wikipedia